Spreadsheet: 2356dacc-60fb-41cd-9075-114092c0521a
Sheet: 3. Inconel

 |  |  |  |  | MD-SLS; Part of SOP
M-spec |  | Linked standards |  | Material / Grade | Dimension limitation | Product | Certificate | Production |  |  | Delivered condition |  |  |  | Chemical composition |  |  |  | Yield & Tensile |  |  |  |  |  |  |  |  |  | Impact energy |  |  |  |  |  |  |  | Hardness (maxim) | [NAME] examination |  |  | Macroetch examination  Acceptance criterias
 |  | NORSOK | Other |  |  |  |  | Raw Material source | Production method | Minimum reduction | Heat treatment procedure | Temp. minimum | Soakingtime | Cooling | Cast / Ladle analysis |  | Product analysis |  | Minimum yield strength |  |  | [NAME] strength |  |  | Ratio | Elongation (minimum) |  |  | Temp | Dimension | Longitudinal J |  |  | Transverse J |  |  |  | Grain size | Duplex grain size | Deleterious phases
 | rev. |  |  |  | m m |  |  |  |  |  |  | ºC | hours |  | Element | Content % | Element | Content % | Dimension m m | KSI | MPa | Dimension m m | KSI | MPa | % | Dimension m m | % | Red. of area | ºC | m m | Average | Single | Lateral expan. | Average | Single | Lateral expan.
M40118 | I |  | API6A718 | UNS N07718  Inconel 718 (150/130) |  |  |  |  |  | 4:1 | 1. Solution annealed  4. Age hardened | 1021 - 1052   774 - 802 | 1 - 2.5   6 - 8 | 2. Air cooled / water quenched  3. Air cooled or faster | Ni (+Co) Cr Fe Mo Nb (+Ta) C Mn Si P S Al Ti Cu Co | 50.0 - 55.0 17.0 - 21.0 Balance 2.80 - 3.30 4.87 - 5.20 [NAME] 0.045 [NAME] 0.35 [NAME] 0.35 [NAME] 0.010 [NAME] 0.010 0.40 - 0.60 0.80 - 1.15 max 0.23 [NAME] 1.00 | Ni (+Co) Cr Fe Mo Nb (+Ta) C Mn Si P S Al Ti Cu Co | 49.65 - 55.35 16.75 - 21.25 Balance 2.75 - 3.40 4.72 - 5.40 [NAME] 0.065 [NAME] 0.38 [NAME] 0.38 [NAME] 0.015 [NAME] 0.013 0.35 - 0.70 0.76 - 1.20 max 0.26 [NAME] 1.03 |  | 130 | 897 |  | 150 | 1035 |  |  | 20 | 25 |  |  |  |  |  |  |  |  | 39 HRC  Final product: 40 HRC
M40407 | F | Compliant to M630 N01, Rev 4 | ASTM B444 ASTM B705  ASTM B366 | Incone. 625  UNS N06625 Grade 1 |  | Tube Pipe (Class1)  Fittings from pipes or tubes | EN 10204 Type 3.1 or higher - Heat treatment condition. |  |  |  | Annealed | 871 (ASTM B366) | x | Rapid air/water | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 |  | 60 | 414 |  | 120 | 827 |  |  | 30 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | F | Compliant to M630 N01, Rev 4 | ASTM B443 ASTM B366 | Incone. 625  UNS N06625; Grade 1 |  | Sheet Strip Fittings from this | EN 10204 Type 3.1 or higher - Heat treatment condition. |  |  |  | Annealed | 871  (ASTM B366) | x | Rapid air/water | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 |  | 60 | 414 |  | 120 | 827 |  |  | 30 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | F | Compliant to M630 N01, Rev 4 | ASTM B443 ASTM B366 | Incone. 625  UNS N06625; Grade 1 | <70mm | Plate Sheet Fittings from this | EN 10204 Type 3.1 or higher - Heat treatment condition. |  |  |  | Annealed | 871  (ASTM B366) | x | Rapid air/water | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 |  | 55 | 379 |  | 110 | 758 |  |  | 30 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | F | Compliant to M630 N01, Rev 4 | ASTM B443 ASTM B366 | Incone. 625  UNS N06625; Grade 1 | <9.5mm | Plate Fittings from this | EN 10204 Type 3.1 or higher - Heat treatment condition. |  |  |  | Annealed | 871  (ASTM B366) | x | Rapid air/water | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 |  | 55 | 379 |  | 110 | 758 |  |  | 30 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | F | Compliant to M630 N01, Rev 4 | ASTM B446 | Incone. 625  UNS N06625 Grade 1 | [NAME] or thickness: 254mm | Bar | EN 10204 Type 3.1 or higher - Heat treatment condition. |  |  |  | Annealed | 871 (ASTM B366) | x |  | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 | <102 102-254 | 60 50 | 414 345 | <102 102-254 | 120 110 | 827 758 |  | <102 102-254 | 30 25 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | F | Compliant to M630 N01, Rev 4 | ASTM B564 | Incone. 625  UNS N06625 | thickness: 254mm | Forgings | EN 10204 Type 3.1 or higher - Heat treatment condition. |  |  |  | Annealed |  | x |  | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 | <102 102-254 | 60 50 | 414 345 | <102 102-254 | 120 110 | 827 758 |  | <102 102-254 | 30 25 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | E | Compliant to M630 N01, Rev 3 | ASTM B444 ASTM B705  ASTM B366 | Incone. 625  UNS N06625 Grade 1 |  | Tube Pipe (Class1)  Fittings from pipes or tubes | EN 10204 Type 3.1 or higher |  |  |  | Annealed | 871 (ASTM B366) | x | Rapid air/water | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 |  | 60 | 414 |  | 120 | 827 |  |  | 30 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | E | Compliant to M630 N01, Rev 3 | ASTM B443 ASTM B366 | Incone. 625  UNS N06625; Grade 1 |  | Sheet Strip Fittings from this | EN 10204 Type 3.1 or higher |  |  |  | Annealed | 871  (ASTM B366) | x | Rapid air/water | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 |  | 60 | 414 |  | 120 | 827 |  |  | 30 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | E | Compliant to M630 N01, Rev 3 | ASTM B443 ASTM B366 | Incone. 625  UNS N06625; Grade 1 | <70mm | Plate Sheet Fittings from this | EN 10204 Type 3.1 or higher |  |  |  | Annealed | 871  (ASTM B366) | x | Rapid air/water | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 |  | 55 | 379 |  | 110 | 758 |  |  | 30 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | E | Compliant to M630 N01, Rev 3 | ASTM B443 ASTM B366 | Incone. 625  UNS N06625; Grade 1 | <9.5mm | Plate Fittings from this | EN 10204 Type 3.1 or higher |  |  |  | Annealed | 871  (ASTM B366) | x | Rapid air/water | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 |  | 55 | 379 |  | 110 | 758 |  |  | 30 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | E | Compliant to M630 N01, Rev 3 | ASTM B446 | Incone. 625  UNS N06625 Grade 1 | [NAME] or thickness: 254mm | Bar | EN 10204 Type 3.1 or higher |  |  |  | Annealed | 871 (ASTM B366) | x |  | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 | <102 102-254 | 60 50 | 414 345 | <102 102-254 | 120 110 | 827 758 |  | <102 102-254 | 30 25 |  |  |  |  |  |  |  |  |  | 35 HRC
M40407 | E | Compliant to M630 N01, Rev 3 | ASTM B564 | Incone. 625  UNS N06625 | thickness: 254mm | Forgings | EN 10204 Type 3.1 or higher |  |  |  | Annealed |  | x |  | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 58 [NAME] 5.0 20.0 - 23.0 8.0 – 10.0  3.15 - 4.15 [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 max 0.40 max 0.40 max 1.0 | Nickel Iron Chromium Molybdenum Columbium & Tantalum Carbon Manganese Silicon Phosphorus Sulfur Aluminum Titanium Cobalt | min 57,65 [NAME] 5.07 19.75 - 23.25 8.0 – 10.0  3.08 - 4.25 max 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 max 0.45 max 0.43 [NAME] 1.03 | <102 102-254 | 60 50 | 414 345 | <102 102-254 | 120 110 | 827 758 |  | <102 102-254 | 30 25 |  |  |  |  |  |  |  |  |  | 35 HRC
M40408 | B |  | ASTM B446 | Incone. 625  UNS N06625, [NAME] |  | [NAME] for hydraulic couplers | EN 10204 Type 3.1 or higher |  |  |  | Solution annealed Stabilization anealed | 1093  982 |  |  | Carbon Manganese Silicon Phosphorus Sulfur Chromium Columbium & Tantalum Cobalt Molybdenum Iron Aluminum Titanium Nickel | [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 20.0 - 23.0  3.15 - 4.15 max 1.0 8.0 – 10.0 [NAME] 5.0 max 0.40 max 0.40 min 58.0 | Carbon Manganese Silicon Phosphorus Sulfur Chromium Columbium & Tantalum Cobalt Molybdenum Iron Aluminum Titanium Nickel | [NAME] 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 19.75 - 23.25  3.00 - 4.30 [NAME] 1.03 7.85 – 10.15 [NAME] 5.07 max 0.45 max 0.43 min 57.65 |  | 45.5 - 60.0 | 314 - 414 |  | 100.5 | 693 |  |  | 30 | 40 |  |  |  |  |  |  |  |  | 230 HBW 20 HRC
M40409 | A |  | ASTM B446  API 6A  ISO 10423 PLS 3 | Incone. 625, grade 1  UNS N06625 |  | [NAME] couplers | EN 10204 Type 3.1 or higher |  |  |  | annealed | min 871 |  |  | Carbon Manganese Silicon Phosphorus Sulfur Chromium Columbium & Tantalum Cobalt Molybdenum Iron Aluminum Titanium Nickel | [NAME] 0.10 [NAME] 0.50 [NAME] 0.50 [NAME] 0.015 max 0.015 20.0 - 23.0  3.15 - 4.15 max 1.0 8.0 – 10.0 max  [NAME] 0.40 max 0.40 min 58.0 | Carbon Manganese Silicon Phosphorus Sulfur Chromium Columbium & Tantalum Cobalt Molybdenum Iron Aluminum Titanium Nickel | [NAME] 0.11 [NAME] 0.53 [NAME] 0.53 max 0.020 [NAME] 0.018 19.75 - 23.25  3.00 - 4.30 [NAME] 1.03 7.85 – 10.15 [NAME] 5.07 max 0.45 max 0.43 min 57.65 |  |  | 414 |  |  | 693 |  |  | 30 | 40 |  |  |  |  |  |  |  |  | 240 - 320 HBN 35 HRC
M40410 | E |  | ASTM B444  ASTM B880 | Inconel 625  Grade 1 | [NAME]: 31.75mm | Tubings | EN 10204 Type 3.1 or higher  Additional reporting required: -Source of raw material -Tube manuf. process -wall thickness tolerances -Heat treatment -Surface preparations | x |  |  | annealed | 871 | x | x | Carbon Manganese Phosphorus Sulfur Silicon Iron Nickel Chromium Molybdenum Titanium Oxygen Aluminium Co* Nb(Cb)+Ta  *not required for routine inspection | [NAME] 0.10 [NAME] 0.50 [NAME] 0.015 max 0.015 [NAME] 0.50 [NAME] 5.0 min. 58.0 20.0 - 23.0 8.0 - 10.0 max 0.40 report [NAME] 0.40 max 1.0 3.15 - 4.15 | Carbon Manganese Phosphorus Sulfur Silicon Iron Nickel Chromium Molybdenum Titanium Oxygen Aluminium Co* Nb(Cb)+Ta  *not required for routine inspection | [NAME] 0.11 [NAME] 0.53 max 0.020 [NAME] 0.018 [NAME] 0.53 [NAME] 5.07 min. 57.65 19.75 - 23.25 7.85 - 10.15 max 0.43 report [NAME] 0.45 [NAME] 1.03 3.00 - 4.30 |  | 60 | 414 |  | 120 | 827 |  |  | 30 |  | DBI may contain Q-spec reference for sharpy requirements |  |  |  |  |  |  |  | 25 HRC
M40902 | P |  | API 6A | Inconel 718 (150/120)  UNS N07718 | Parts with [NAME] | tubing hangers & bar stocks |  |  |  | 4:1 | 1. solution annealed    3. age hardened | 1021 - 1052    774 - 802 | 1 - 2.5 hours    6 - 8 hours | 2. air, inert gas, polymer, oil or water   4. air cool or faster | Ni (+Co) Cr Fe Mo Cb (+Ta) C Mn Si P S Al Ti Cu Co | 50.0 - 55.0 17.0 - 21.0 Balance 2.80 - 3.30 4.75 - 5.20 [NAME] 0.045 [NAME] 0.35 [NAME] 0.35 [NAME] 0.010 [NAME] 0.010 0.20 - 0.80 0.80 - 1.15 max 0.23 [NAME] 1.00 |  |  |  | 120 | 828 |  | 150 | 1035 |  |  | 20 | 25 | -60 | <254  >254 | 47  41 | 41  37 |  |  |  |  | Before machining:  39 HRC  Final product: 40HRC
M40910 | N |  | API 6A API 6A718 | (120K) UNS N07718 |  | tubing hangers stems  other critical, high load bearing components | EN 10204 Type 3.1 or higher  Additional information: -Chemical analysis results -Melt practice utilized -Name of melt source -Name of company performing the hot working operations (if different from melt source) -Name of company performing the heat treatment (if different from melt source) -Total hot work reduction ratio -Actual heat treatment times and temperatures and cooling media -Name of test laboratory -Statement that the material complies with the requirements of the macroetch examination -Predominant grain size -Statement of compliance with topological duplex grain size testing requirement -Statement that the material complies with the requirements of the metallographic examination for deleterious phases (note section 2.3 requirement when applicable) In addition, a complete set of legible photomicrographs taken at all three referenced locations (at 100X and 500X) is required. -Tensile test results -Impact test temperature, orientation, and results -Hardness test results | x | Alternative 1: EF AOD/VOD VAR (VAR)  Alternative 2: VIM ESR/VAR (ESR/EFR/VAR) | 4:1 | 1. solution annealed    3. age hardened | 1021 - 1052    774 - 802 | 1 - 2.5 hours    6 - 8 hours | 2. air, inert gas, polymer, oil or water   4. air cool or faster | [NAME] (Cb) + Ta Mo Ti Al C Co Mn Si P S B Cu Pb Se Bi Ca Mg | 50.0 - 55.0 17.0 - 21.0 Balance 4.87 - 5.20 2.80 - 3.30 0.80 - 1.15 0.40 - 0.60 [NAME] 0.045 [NAME] 1.00 [NAME] 0.35 [NAME] 0.35 [NAME] 0.010 [NAME] 0.010 [NAME] 60 ppm [NAME] 0.23 [NAME] 10 ppm [NAME] ppm [NAME] 0.5 ppm [NAME] 30 ppm [NAME] 60 ppm | [NAME] (Cb) + Ta Mo Ti Al C Co Mn Si P S B Cu Pb Se Bi Ca Mg | 49.65 - 55.35 16.75 - 21.25 Balance 4.72 - 5.40 2.75 - 3.40 0.76 - 1.20 0.35 - 0.70 [NAME] 0.055 [NAME] 1.03 [NAME] 0.38 [NAME] 0.38 [NAME] 0.015 [NAME] 0.013 [NAME] 80 ppm [NAME] 0.26 [NAME] 30 ppm [NAME] ppm [NAME] 0.5 ppm [NAME] 30 ppm [NAME] 160 ppm |  | 120 - 145 | 827 - 1000 |  | 150 | 1034 |  | <254 >254 | 20 | 35 25 | <-60 | <76 76 - 254 >254 | 68 | 61 | 0.38 | 47 41 | 41 37 | 0.38 0.38 | 298 - 363 HBW 32 - 40 HRC | No 2 or finer In accordance with: ASTM E 112 | Not permitted | a) Free from continuous networks of secondary phases along grain boundaries or other unusual microstructural features  b) Free from continuous networks of acicular delta phase  c) No laves phase | Class 1 to 4
M40910 | L |  | API 6A API 6A718 | (120K) UNS N07718 |  | tubing hangers stems  other critical, high load bearing components | EN 10204 Type 3.1 or higher  Additional information: -Name melt source -Name company performing the hot working operations -Name company performing the heat treatment  -Name test laboratory [NAME] set of legible photomicrographs taken at all three referenced locations (at 100X and 500X) is required. | x | Alternative 1: EF AOD/VOD VAR (VAR)  Alternative 2: VIM ESR/VAR (ESR/EFR/VAR) | 4:1 | 1. solution annealed    3. age hardened | 1021 - 1052    774 - 802 | 1 - 2.5 hours    6 - 8 hours | 2. air, inert gas, polymer, oil or water   4. air cool or faster | [NAME] (Cb) + Ta Mo Ti Al C Co Mn Si P S B Cu Pb Se Bi Ca Mg | 50.0 - 55.0 17.0 - 21.0 Balance 4.87 - 5.20 2.80 - 3.30 0.80 - 1.15 0.40 - 0.60 [NAME] 0.045 [NAME] 1.00 [NAME] 0.35 [NAME] 0.35 [NAME] 0.010 [NAME] 0.010 [NAME] 60 ppm [NAME] 0.23 [NAME] 10 ppm [NAME] ppm [NAME] 0.5 ppm [NAME] 30 ppm [NAME] 60 ppm | [NAME] (Cb) + Ta Mo Ti Al C Co Mn Si P S B Cu Pb Se Bi Ca Mg | 49.65 - 55.35 16.75 - 21.25 Balance 4.72 - 5.40 2.75 - 3.40 0.76 - 1.20 0.35 - 0.70 [NAME] 0.055 [NAME] 1.03 [NAME] 0.38 [NAME] 0.38 [NAME] 0.015 [NAME] 0.013 [NAME] 80 ppm [NAME] 0.26 [NAME] 30 ppm [NAME] ppm [NAME] 0.5 ppm [NAME] 30 ppm [NAME] 160 ppm |  | 120 - 145 | 827 - 1000 |  | 150 | 1034 |  | <254 >254 | 20 | 35 25 | <-60 | <76 76 - 254 >254 | 68 | 61 | 0.38 | 47 41 | 41 37 | 0.38 0.38 | 298 - 363 HBW 32 - 40 HRC | No 2 or finer | Not permitted | a) Free from continuous networks of secondary phases along grain boundaries or other unusual microstructural features  b) Free from continuous networks of acicular delta phase  c) No laves phase | Class 1 to 4